Polymerization in Liquid Crystal Medium: Preparation of Polythiophene Derivatives Bearing a Bulky Pyrimidine Substituent

We carried out polycondensation of monomers bearing a bulky pyrimidine substituent in a liquid crystal solvent. The resultant polymers formed nematic liquid crystals. The polymers prepared in liquid crystals had higher coplanarity than the polymers prepared in toluene. This can be due to the fact that the ordered medium of the liquid crystal produces an aggregated structure with well-developed -stacking between the main chains. The present results demonstrated that polymerization of bulky monomers is possible in liquid crystal solvents.


Introduction
Liquid crystals (LCs) have fluidity and crystal-like order [112].Previous studies reported syntheses of polythiophenes bearing alkyl groups in LCs as anisotropic media [13].The resultant polymers possessed the structural order derived from the LC media employed for the polymerization.The polymerization process was influenced by the ordered structures of LCs and resulted in formation of LC order for the resultant polymers.Such studies have reported successful polymerization in the LC OPEN ACCESS media from monomers that displayed good affinity towards LCs.Polymerization in LC media may require a certain combination of molecular forms of the LCs and monomers.
In the present study, following from the successful polymerization of the aromatic main chain type polymer bearing flexible alkyl group, we conducted polycondensation of monomers bearing a bulky substituent in LCs to explore the possibility of polymerization in LC.Thermotropic behavior of the polymers thus obtained is investigated with differential scanning calorimetry (DSC) and visual observation of the optical textures is carried out with polarizing optical microscopy (POM).Furthermore, optical properties such as optical absorption and photoluminescence are discussed based on consideration of aggregation derived from inter-chain interaction of the polymers.The results of this study may open the possibility of various polymerization reactions in liquid crystals as reaction media.

Materials and methods
All syntheses except the Williamson etherification reaction in the present study were conducted under argon atmosphere.4-(5-Nonyl-pyrimidine-2-yl)-phenol (compound 1) was provided by Midori Chemicals and used for side chains of polymers.2,5-Bis-trimethyl-stannyl thiophene and 5,5'-bis(trimethylstannyl)-2,2'-bithiophene were synthesized by a previously reported method [16]. 1 H-NMR spectra were measured with JNM-ECS 400 (JEOL) and EX-270 (JEOL) NMR spectrometers.CDCl 3 was employed for the NMR solvent.Chemical shifts are represented in parts per million downfield from tetramethylsilane (TMS) as an internal standard. 1H- 13 C hetero-nuclear multiple quantum coherence (HMQC) NMR were measured with an AVANCE-500 Spectrometer (Bruker).Infrared absorption spectra were measured with an FT/IR-300 spectrometer (JASCO).UV-vis absorption spectra of the polymers in chloroform were measured with a V-630 UV-vis optical absorption spectrometer (JASCO).Photoluminescence spectra of the polymers in chloroform were measured with an F-4500 fluorescence spectrophotometer (HITACHI).Optical textures of the LC and the polymers were observed with an ECLIPSE LV100 polarizing optical microscope (Nikon) equipped with a TH-600PM (Linkam) thermo control stage.The samples were sandwiched between two thin glass slides for the POM observations.Differential scanning calorimetry (DSC) analysis was conducted with a DSC6200 (SEIKO Instruments).

Synthesis of cholesteric liquid crystal medium
A cholesteric liquid crystal medium, (R)-LC, was synthesized according to the literature procedure [13].Scheme 1 shows the chemical structure of the (R)-LC.The (R)-LC has a mesogen which consists of three-ring and flexible alkyl chains at both ends of the molecule, which allows the formation of the LC phase under appropriate conditions.
Liquid crystals having three-ring aromatic cores tend to be in the liquid crystal state at high temperatures (>100 °C).In fact, the (R)-LC exhibits a liquid crystal phase at 78-137 °C.Therefore, (R)-LC can be employed as the reaction medium for the Migita-Kosugi-Stille type polycondensation reactions, which require high reaction temperatures (>100 °C).Scheme 1.Chemical structure of (R)-LC.
Gel permeation chromatography (GPC) relative to polystyrene reference was carried out to estimate the molecular weight of the polymers.The number-average molecular weights (M n ) of P1T, P2T, P1LC, and P2LC ranged from 3,400 to 4,700.The weight-average molecular weights (M w ) of P1T, P2T, P1LC, and P2LC ranged from 5,700 to 6,900.The synthesis yields of P1T and P2T were 90% and 84%, respectively, while the yields of P1LC and P2LC were somewhat low, namely 46% and 66%, respectively.This may be due to the fact that the steric hindrance between the (R)-LC molecules and the monomers resulted in depression of the polymerization activity for P1LC and P2LC.The low molecular mass fractions of P1LC and P2LC were removed by purification resulting in the low synthesis yield.

Infrared absorption spectra
Figure 1 shows infrared (IR) absorption spectra of (R)-LC, P1LC, P2LC, P1T, and P2T.In the IR absorption spectra, P1LC and P1T exhibited the same features.Similarly, P2LC and P2T exhibited the same spectral shape.The GPC and IR absorption results suggested that the polymerization in the (R)-LC was successfully conducted.

Ultraviolet-visible absorption and photoluminescence spectra
Figure 2 shows ultraviolet-visible (UV-vis) absorption spectra for the polymers in chloroform solutions.All polymers exhibited two absorption bands.The absorption bands of the polymers at short wavelengths were located at almost the same position (284 nm), which is characteristic of the * transition of phenyl pyrimidine moiety in the side chains.On the other hand, the absorption bands at long wavelengths are attributable to the * transition in the conjugated main chains.The maximum absorption wavelength (λ max ) at 389 nm for the P1LC is 5 nm longer than that for the P1T (384 nm).Similarly, λ max for P2LC at 425 nm is 13 nm longer than that for P2T (412 nm).These red shifts indicated a development of -stacking between the polymers prepared in (R)-LC.Here, an anisotropic propagation of the polymers may occur along the liquid crystalline order during the polymerization process in the (R)-LC medium.The thiophene units may stack in the narrow space between the liquid crystal molecules during the polymerization.The absorption bands of P2LC and P2T were located at longer wavelengths than those of P1LC and P1T because the introduction of a bithiophene unit into the main chain without the side chain provides an ample space between the substituents, and the space may improve coplanarity of the polymer.Besides, an increase in the ratio of the thiophene units leads to lower energy bandgap of the polymers, because in general, polythiophenes have lower energy bandgaps than the poly-p-phenylenes.Here, effective conjugation length of the present polymers may not be highly developed compared to non-substituted polyacetylene.Furthermore, molecular weights of the polymers are almost the same range.Therefore, in the present stage we do not consider dependence of molecular weight for the optical absorption results.
Figure 3 shows optical absorption spectra of P2T and P2LC at low concentration in chloroform solution (P2T, C = 9.6 × 10 −6 M; P2LC, C = 7.5 × 10 −6 M).The absorption maximum of P2LC displays 12 nm longer than that of P2T.Further, the absorption intensity is stronger than that of P2T.This may be due to the fact that an aggregation produced in the liquid crystal medium allows development of coplanarity between adjacent monomer repeat units in the main chain.The normalized intensity of the polymers decreased with concentration.The intensities of P2LC are stronger than that of P2T at each concentration.The intensity maximum of the P2LC locates at long wavelengths compared to P2T.This may be due to the fact that restricted space of LC medium during the polymerization improves molecular packing between the main chains and affords good -stacking to form.The -stacking locks the aggregation for improvement of coplanarity.The red-shift observed for P2LC is due to development of electronic delocalization on the main chain.The result of excitation spectra is consistent with the absorption spectra of the polymers at low concentration.mg / mL 12 x 10 -3 mg / mL 18 x 10 -3 mg / mL 24 x 10 -3 mg / mL 425 nm

C
Figure 5 shows photoluminescence (PL) spectra for P2T and P2LC at low concentration in chloroform solution.The PL intensity of P2LC is stronger than that of P2T.Also, the PL maximum value of P2LC is located at slightly longer wavelengths (2 nm) compared to P2T.This result suggests that the aggregation produced by the liquid crystal medium during the polymerization reaction allows improvement of emission of the polymer.The color of the texture derived from optical retardation, and it depends on each condition of POM observations (i.e., sample thickness in the cell or substrate state).The optical textures demonstrate that the helical axis of all of the samples locates normal direction to the substrate (this is a characteristic of Grandjean texture).

Phase transition
Phase transition temperatures for the polymers thus prepared were determined with both differential scanning calorimetry (DSC) (Figure 8) and POM observations.The DSC signals did not display high resolution because the enthalpy change involves both phase transition of the side chain and the main chain.Furthermore, the dispersion of the molecular weight of the main chain in the polymer complicates the transition.
All polymers exhibited blushes under the POM, which is typical of Schlieren textures of nematic LC (NLC) order.Both polymers prepared in isotropic solution (toluene) and polymers prepared in LC show nematic phase.The polymer aggregation is released with temperature during the heating process, and the polymers form liquid crystal order.Continuously, the phase transition from LC (mesophase) to isotropic state (liquid phase) occurs in the heating process.Note that the mono-1 shows no LC.On the other hand, the corresponding polymer exhibits thermotropic liquid crystallinity.This phenomenon can be referred to as the polymer effect, because the polymerization produces liquid crystallinity in this system.Sequential arrangement of the side chain attached onto the main chain and the rigid form of the main chain of polymers allow formation of polymer LC.
The transition temperatures from isotropic phase to LC phase of P1T, P2T, and P1LC were in the range of 135160 °C, while the transition temperature from isotropic phase to LC phase of P2LC was 220 °C.This high phase transition temperature of P2LC suggested that P2LC may have a higher molecular weight than that of the other polymers.Alternatively, P2LC may have a tight aggregated structure.The GPC measurement of P2LC estimated a lower molecular weight fraction because the polymer solution was filtered using a microporous membrane to exclude the insoluble fraction.This procedure is required for GPC measurements.The optical textures of P1LC (at 120 °C), P2LC (at 200 °C), P1T (at 130 °C), and P2T (at 120 °C) were observed with the POM (Figures 9 and 10).
Liquid crystallinity of polymers can be derived from the orientation of the main chain.Here, the main chain plays a role of a mesogen with the cooperation of side chain LC group.This may be referred to as super mesogen form.This is because both the main chain and the side chain did not independently exhibit liquid crystallinity.The super mesogen form was observed for the main chain-side chain type polymers in the previous study [18].XRD measurements can further confirm the structure of the polymer, and may display broad signal (hallow) such as typical nematic phase.The plausible structure is shown in Figure 11.The texture of the polymer (Schlieren, nematic) is different from that of the (R)-LC medium (Grandjean, cholesteric).This result supports the fact that the polymer contains no LC medium.If the sample contains some cholesteric molecules, the polymer would show cholesteric phase because a small amount of chiral compounds induces cholesteric phase in the entire system.A set of polymerization results in this study demonstrated that the reaction in the liquid crystal medium successfully produced polymers with bulky pyrimidine LC group.

Conclusions
We successfully carried out the polycondensation of aromatic monomers with the bulky pyrimidine substituent in a LC as the polymerization solvent.The resultant polymers show nematic LCs accompanied by the formation of super mesogens.The polymers thus prepared in (R)-LC have relatively long effective -conjugation length due to development of coplanarity derived from -stacking.The results of this study demonstrated the possibility of conducting various polymerization reactions in ordered solvents.

Figure 3 .Figure 4
Figure 3. UV-vis absorption spectra for P2T (yellow-green line) and P2LC (purple line) at low concentration in chloroform solutions.

Figure 6 .
Figure 6.Polarizing optical microscopic (POM) images of the reaction mixture of P1LC before polymerization (a) and P1LC after polymerization (b).

Figure 7 .
Figure 7. POM images of the reaction mixture of P2LC before polymerization (a) and P2LC after polymerization (b).

Figure 11 .
Figure 11.A plausible structure of the main chain and side chain cooperation LC system (super mesogen).